Tuning of Quantum Interference in Top-Gated...
Embed Size (px)
Transcript of Tuning of Quantum Interference in Top-Gated...
•Hall bar (300 μm x 50 μm) •Epitaxial graphene layer grown on the Si face of a SiC (0001) wafer. •The dielectric: Hydrogen Silsequioxane (140 nm) + SiO2 (40 nm). • Cr/Au (10/180 nm) top gate
• Data normalized to (Rxx-R0)/R02 • Fit to extract A= Kee ln(kBT τtr /ħ) • Good fit for all datasets. The B-range depends on T and n, being limited by the onset of QH effect. • We presented a systematic analysis of magnetotransport properties in
epitaxial graphene grown on the Si-terminated face of SiC. •We describe EEI in graphene with the current theory for disordered systems, and we find an unexpected dependence of the interaction parameter Kee on carrier density. • From fits of the quantum interference correction, we obtain the scattering times as a function of carrier density. The dephasing and intervalley times are almost constant, while the intravalley scattering time shows a peculiar dependence on density, which is different from the one due to the sole warping term. • Our results stress the role of charge density in determining quantum interference and EEI, and the necessity of further investigation of its impact on
the low-field magnetoresistance of graphene devices.
• density-mobility diagram (Ref. ) • I (3.75·1011 cm-2), II (1,43·1011 cm-2), •III (2.02·1010 cm-2), IV (-2.03 ·1010 cm-2)
• Chirality, due to the peculiar Dirac-like energy diagram, produces destructive interference by adding a Berry phase π, thus Weak Anti Localization (WAL) is expected.
Scattering times: τφ≈ τiv » τ*
EXPERIMENTAL DETAILS QUANTUM INTERFERENCE
• Half-integer QH effect monolayer graphene • Charge Neutrality Point: VTG≈-27 V
Andrea Iagallo,1 Shinichi Tanabe,2 Stefano Roddaro,1, 3Makoto Takamura,2 Hiroki Hibino,2
Stefan Heun,1 and Fabio Beltram1
1NEST, Istituto Nanoscienze - CNR and Scuola Normale Superiore, Piazza San Silvestro 12, 56127 Pisa, Italy 2NTT Basic Research Laboratories, NTT Corporation, 3-1 Morinosato Wakamiya, Atsugi, Kanagawa, Japan 3Istituto Officina dei Materiali CNR, Laboratorio TASC, 34149 Trieste, Italy
We report on quantum interference measurements in top-gated Hall bars of graphene epitaxially grown on the Si face of SiC. We perform a systematic study of the quantum corrections to the magnetoresistance due to quantum interference of quasiparticles and electron-electron interaction, by varying the temperature and charge density. We analyze the contribution of the different scattering mechanisms affecting the quantum interference in the 2·1010 - 3.75·1011 cm-2 density range and find, besides a transition from Weak Localization to Weak Anti Localization, a signicant infuence of the charge density on the intravalley scattering time. We also observe a modulation of the electron-electron interaction as a function of charge density not accounted for by present theory. Our results stress the role of SiC-based devices as a promising technology for graphene coherent electronics.
Tuning of Quantum Interference in Top-Gated Graphene
 S. Tanabe, Y. Sekine, H. Kageshima, M. Nagase, and H. Hibino, Phys. Rev. B 84, 115458 (2011).  B. Altshuler and A. Aronov, Electron-Electron Interaction in Disordered Systems (North Holland, Amsterdam, 1985).  E. McCann, K. Kechedzhi, V. I. Fal'ko, H. Suzuura, T. Ando, and B. L. Altshuler, Phys. Rev. Lett. 97, 146805 (2006).  A. M. R. Baker, J. A. Alexander-Webber, T. Altebaeumer, T. J. B. M. Janssen, A. Tzalenchuk, S. Lara-Avila, S. Kubatkin, R. Yakimova, C.-T. Lin, L.-J. Li, and R. J. Nicholas, Phys. Rev. B 86, 235441 (2012).
•Aharonov-Altshuler interaction: Coulomb interaction enhanced in diffusive regime by long interaction time :
•Parabolic in B: • momentum relaxation time τtr≈0.01-0.02 ps •Kee: e-e interaction parameter, depending linearly on the number of channels c participating in the interaction.
A ~ Kee ~ c (number of channels) •Constant slope of A (at each density) constant c
• Variation of channel number c with quasiparticle density.
• Intervalley scattering decreases quasiparticle coherence. Suppression of WL and WAL. • Intravalley scattering preserves coherence, but not chirality. Restoration of WL.
n behaviour •τφ: , τiv weak dependence •τ
* : decreasing with n. Weaker dependence
than the sole warping term τw~n-2
• we find τ* ~n-1/2 (see also Ref. )
T behaviour •τφ: T-1 (for T>4 K), saturation (for T